CHAPTER 3 — AN ATOMISTIC-CONTINUUM STUDY OF POINT DEFECTS
Accurate modeling of coupled stress-diffusion problems requires that the effect of
stress on the diffusivity and chemical potential of defects and dopants be quantified.
Although the aggregate effects of stress on diffusion are readily observable, it is
difficult to experimentally measure stress-induced changes in diffusivity and chemical
potential. Despite these difficulties a number of careful measurements have been made
regarding the effect of stress on diffusivities in model semiconductor systems [Zhao et
al. 1999A, Zhao et al. 1999B], and the formation energies of vacancies have been
measured in metals [Simmons and Balluffy 1960]. Due to the experimental challenges,
an extensive literature has emerged regarding the numerical calculation of the formation
energies of these defects using atomistic simulation [Antonelli et al. 1998, Antonelli and
Bernholc 1989, Puska et al. 1998, Zywietz et al. 1998, Song et al. 1993, Tang et al.
1997, Al-Mushadani and Needs 2003]. Although early work used empirical potentials,
more recent work has focused on the application of tight-binding and ab initio methods
which are more accurate in modeling the alterations in bonding that occur at the defect.
These calculations have been limited to a few hundred atoms due to the computational
requirements of these methods.
This chapter addresses a number of unresolved issues in the application of atomistic
simulations to accurately extract formation volumes and stress fields of point defects. In
order to illustrate the methods that can be used to calculate the appropriate
thermodynamic and elastic parameters from atomistic data we have performed
calculations regarding a simple model point-defect, a vacancy in the Stillinger Weber
[Stillinger and Weber 1985] model of silicon. An empirical model of silicon bonding
was employed because it allows the exploration of a much larger range of system sizes
than would have been possible using a more accurate model. Using an empirical
potential precludes a quantitatively accurate measure of, for example, the formation
volume of a vacancy in silicon since this model does not properly model the change in
bonding that occurs at the vacancy. However the larger system sizes accessible via such
a method are necessary to demonstrate a new technique for accurately calculating the
prediction that does arise from the Stillinger Weber model of silicon and, by extension,
in other atomistic potentials. This is critical since our goal is to make firm connections
between the atomistic data and continuum concepts that, as we shall show, are not yet
convergent on the scale of current ab initio calculations. This work paves the way for a
multiscale modeling technique in which ab intio, atomistic and continuum concepts are
used together to extract such quantities with predictive accuracy.
2) Formation volume
Chapter 1 introduced the free energy of activation which quantifies the effect of an
external stress on the formation and migration of a defect in a crystal. This section
focuses on the formation energy which is a part of the activation energy. The formation
free energy determines the number of defects in the crystal. It comes from a change in
internal energy Ef, a change in entropy Sf (usually small) and a work term,
G f = E f − TS f − σ : V f = E f − TS f − Wext , (3.1)
where Vf is a tensor describing the change in volume and shape of the system and Wext
is the work done by σ on the system. The derivative of the free energy with respect to
the externally applied stress provides the fundamental definition of this volume term.
Equation (3.1) shows that the free energy depends on the pressure through the work.
However it may also be indirectly pressure-dependent if the internal energy depends on
the pressure. The internal energy of formation can be split into two parts, an elastic part,
EfLE, accounting for the elastic energy related to the crystal relaxation around the
vacancy and a core energy, Efcore, arising from broken bonds.
H f = E fLE + E fcore − σ : V f (3.2)
While the elastic part can be treated using linear elasticity, the core energy part must be
treated atomistically. In linear elasticity, there is no interaction between internal and
external stresses [Eshelby 1961] therefore ELE does not depend on σ. The core energy
comes from the broken bonds and is therefore expected to be independent of the
pressure. Therefore the only dependence of H upon σ is from the σV term.
The formation volume is the change of volume of a system upon introduction of a
defect. Let system 1 be a perfect crystal under some external stress σ and system 2 the
same crystal under the same external stress σ to which a defect was added. The
formation volume Vf is the difference of volumes of the two systems. Similarly Ef is the
difference in internal energy between the two systems. The external stress contributes to
the internal energy through the elastic energy EfLE, but since these two systems are
under the same stress these contributions cancel out.
As described in chapter 1, the stress dependence of the formation of defects is of
technological importance. This dependence is captured by the formation volume. If, for
FIG. 3.1: Vacancy as an Eshelby inclusion. Part of the medium is removed (1).
Its volume is decreased by Vt (2). It is reinserted into the medium (3).
a given defect, Vf is 0 the concentration of this defect does not depend on the external
stress. If a defect A has a positive formation volume and a defect B has a negative
formation volume, under compression, the number of B defects increases and the
number of A defects decreases. Under tension the number of A defects increases and the
number of B defects decreases. If part of a film or of a device is under tension and
another part is compressive, a segregation of species A and B can result. Therefore the
behavior of the dopants/defects under stress depends upon the sign and magnitude of Vf.
Although the origin of the formation volume is atomistic in nature, a formulation in
the context of continuum elasticity has also been adapted to interpret Vf in terms of an
internal transformation of the material. This picture assumes the existence of a
continuum defect that has a reference state independent of the surrounding crystal.
Figure 3.1 shows the theoretical construction that would create such an “Eshelby
inclusion” [Eshelby 1961]: material is removed from a continuous medium, the removed
material undergoes a transformation described by a tensor Vt, then it is reinserted into
the medium. Upon reinsertion into the medium there will be elastic distortions both of
the inclusion and of the crystal around it. It is worth noting that the change in volume
(and potentially of shape) described by Vt is the change in shape and volume of the
inclusion when not interacting elastically with the surrounding material. Thus Vt is not
equal to the distortion of the inclusion because this distortion is affected by the elasticity
of the medium. If the volume of the part of the medium which is removed decreases in
step 2, upon reinsertion it will make the medium shrink. It is therefore called a center of
contraction. If an external stress is applied, there will be an interaction between the
center of contraction and the crystal.
The tensor, Vt, is calculated by assuming a homogeneous strain over the transformed
material, and multiplying this strain by the initial, scalar volume of this region. When a
vacancy is to be represented by this continuum analogue, the scalar volume is often
assumed to be the atomic volume, Ω. In this interpretation the external work is exactly
balanced by the work done to transform the inclusion against the external stress, σ, and
can be shown to result in an external work Wext = σ : Vt. When evaluated at the
boundary the strain field results in the change in volume and shape, Vt, that must be
equivalent to Vf to be consistent with the thermodynamic formulation. However, the
arguments leading to Wext = σ : Vt are meaningful only within continuum elasticity
[Eshelby 1961], a theory that loses validity in the neighborhood of the defect. While the
interpretation of Vt as a continuum transformation is not physically relevant for a point
defect, this transformation can be used to calculate the elastic strain and stress fields in
the vicinity of the transformation if Vf is known.
FIG. 3.2: Dipole representation of the point defect.
It is possible to extend the Eshelby inclusion model to point defects such as
vacancies by shrinking the inclusion to a point. The elastic field of a vacancy is then
modeled using a force dipole. This dipole is similar to an electric dipole. It is composed
of forces an infinitesimally small distance apart. Since forces can act in any direction
and be separated by a displacement in any direction the dipole is most generally
represented by a tensor. This model can work even for a defect with an anisotropic
stress field. When the dipole is proportional to the identity matrix it represents an
isotropic center of contraction or expansion.
If three force pairs f1, f2 and f3 are applied at three points d1, d2 and d3 away from the
vacancy (Fig. 3.2), the dipole is defined as [de Graeve 2002]
D = ∑ fi ⊗ di . (3.3)
These three vectors do not have to be orthogonal, they only have to be a basis of 3D
space. Far away, when r >> d, the force field is
F(r ) = −D.∇ r [δ(r )] . (3.4)
For the sake of simplicity, the origin of r is taken to be at the defect. The analytical form
of Eq. (3.4) ensures that the sum of forces is 0. The sum of moments is
∫ r × F(r ) = (D 32 − D 23 ) e1 + (D13 − D 31 ) e 2 + (D 21 − D12 ) e 3 (3.5)
where Dij is the (i, j) component of the tensor D and (ei) are unit vectors. Equilibrium
requires that Eq. (3.5) be equal to 0 and thus that D be symmetric. The eigenvalues of a
symmetric matrix are real and its eigenvectors can be chosen to be orthonormal. The
dipole tensor can thus be written as
⎛ f1′ d1 0 0 ⎞
D = R.D′.R = R. ⎜ 0-1
f 2 d ′2 0 ⎟ .R -1 (3.6)
⎜ 0 0 f 3 d′ ⎟
where R is a rotation matrix.
Having characterized the force distribution associated with the defect the
displacement field can be derived from the elastic solution in a generalized elastic
medium. The most general derivation of this kind is to compose the solution from the
Green’s function that satisfies the equation
∂ 2 G km (r )
C ijkl + δ im δ(r ) = 0 . (3.7)
∂x j ∂x i
Here Cijkl is the elastic modulus tensor of the solid and Gkm is the tensorial elastic
Green’s function. Once the Green’s function is derived from Eq. (3.7), the displacement
field can be expressed
u(r ) = −∇ r [G (r ).D] . (3.8)
The resulting solution can be calculated from the expression [Barnett 1972, de Graeve
∫ [− (M ) ]
u(r ) = 2
.D.r + (J.D.z ) dψ .
Here M-1 is the inverse of the matrix M, where M is defined by
M ir (z ) = C ijrs z j z s , (3.10)
r is given by
r= , (3.11)
J is such that2
J ij = C kpln M ik M lj (z p rn + z n rp )
ˆ ˆ (3.12)
and z is
⎛ cosψ sinθ + sinψ cosθ cosϕ ⎞
z = ⎜ − cosψ cosθ + sinψ sinθ cosϕ ⎟ (3.13)
⎜ − sinψ sinϕ ⎟
where θ and ϕ are the polar and azimuthal angles of r. The strain is
∫ [2(M ) ]
ε(r ) = .D.r ⊗ r − 2(J.D.r ⊗ z + J.D.z ⊗ r ) + (A.D.z ⊗ z ) dψ
-1 s s s
ˆ ˆ ˆ ˆ
where the “s” stands for symmetric, i.e.
A + At
As = . (3.15)
If the medium is isotropic, Eq. (3.9) can be written in a closed form [Hirth and Lothe
u(r ) = − 2
4π C11 r
and the strains are
ε rr =
∂r 2π C11 r
J is used here instead of F (notation used by Barnett) to avoid confusion with forces.
ε θθ = ε ϕϕ =
r 4π C11 r
The stresses then are
C11 − C12 (D.r ).r
σ rr = C11 ε rr + C12 ε θθ + C12 ε ϕϕ = 3
2 π C11 r
C11 − C12 (D.r ).r
σ θθ = σ ϕϕ = C12 ε rr + (C11 + C12 ) ε θθ = − 3
2 2π C11 r
C11 − C12
As we assume isotropy, is equal to C44. So (keeping in mind that C44 actually
C11 − C12
means “isotropic C44”, i.e. ), we can write
C 44 (D.r ).r
σ rr = (3.21)
C11 π r 3
C 44 (D.r ).r
σ θθ = σ ϕϕ = − . (3.22)
C11 2π r 3
The radial force on an area A a distance r from the defect is then
A C 44 (D.r ).r
F = σ rr A = (3.23)
π C11 r 3
where A is the surface of the atom on which the force applies.
A priori, the dipole may not be enough to represent any point defect and higher order
terms, such as a quadrupole, may be necessary. However, results for the vacancy show
that the dipole is a good description of this point defect. It is possible that more
complicated defects or clusters require a quadrupole term. In any case, the contribution
of higher order terms to the stress field should die off faster than the dipole and may be
noticeable only close to the defect.
3) Calculating the formation volume
a) Change of volume of the simulation cell
The most common method used to extract the formation volumes of defects has been
the direct measurement of the change in volume of the relaxed supercell upon the
introduction of the defect [Zhao et al. 1999A, Zhao et al. 1999B]. This is a rigorously
correct method of calculating the formation volume given two assumptions: that the
core energy, defined in Eq. (3.2), is not pressure dependent and that the supercell size is
sufficiently large such that defect-defect interactions have a negligible effect on the
elastic relaxation of the cell. The former is typically a good assumption. The latter may
not always be a good assumption for the small supercell sizes typically simulated by ab
initio calculation. The vacancy-vacancy interaction will be shown to have a negligible
effect even for small systems; however this may not be the case for other defects, in
particular the anisotropic ones.
b) Obtaining the dipole from positions and forces
Although the above elastic analysis provides a means to calculate the displacement
and stress fields around a defect of elastic dipole D, it does not provide a means to
extract this dipole value. The dipole value can however be extracted from the forces on
the atoms surrounding the defect. In an isotropic medium, the radial force expected on
atom n from the dipole is
C 44 D . r n
F′ n = A n (3.24)
C11 π r n 4
where rn is the position of atom n relative to the center of the defect. This provides the
forces as a function of the dipole. In fact the dipole is unknown and the forces can be
obtained form atomistics. Equation (3.24) must be somehow inverted to have the dipole
as a function of the forces. We define the vector ∆n as the difference between the actual
force on atom n, Fn (obtained from atomistic simulations) and the radial force expected
from the dipole in an isotropic medium, F’n,
C 44 D . r n
∆ n = F n − F′ n = F n − A n . (3.25)
C11 π r n 4
We then define the scalar ∆ by
⎜ C D.rn ⎟
∆2 = ∑ ∆ n ( ) 2
= ∑ ⎜ F n − A n 44
C11 π r n 4 ⎟ . (3.26)
n n ⎜ ⎟
If the representation of a vacancy (as a center of contraction) in elasticity and its
atomistic counterpart were in perfect correspondence, ∆ would be 0. But since D has 6
components, while there are 3n forces and 3n positions it is not generally possible to
find a D that satisfies the condition ∆ = 0. We therefore pick the tensor D which
minimizes ∆2. To this end, we calculate the derivatives of ∆2 with respect to the
components of D
⎛ Fn r n D ik rkn r jn ⎞
∂∆ 2 2 C 44 ⎜ i j n C 44 ⎟
∂D ij π C11
∑A ⎜− n 4 + ∑A C
= 0. (3.27)
k 11 π rn ⎠
Fin r jn n n
C 44 D ik rk r j
= ∑∑ A ( ) n 2
C11 π r n 8
n rn n k
Fn ⊗ rn
X = ∑ An 4
1 C 44 rn ⊗ rn
∑ (A )n 2
Eq. (3.28) can be rewritten as [de Graeve 2002]
D = X.Y-1. (3.31)
Equation (3.31) provides a means to calculate the value of the dipole using the
positions of and the forces on the atoms from atomistics. It is a closed form solution for
a generalized defect in an isotropic medium. We will take the sum in Eqs. (3.29) and
(3.30) to be over atoms on a cubic shell, as shown in Fig. 3.3.
FIG. 3.3: Cubic shells used to
calculate the dipole.
From Eqs. (3.29) and (3.30) the forces on atoms are needed to calculate the dipole.
However, at equilibrium the net force on any atom is zero. Figure 3.4 shows, in black,
an atom belonging to the shell. If all atoms within the shell (white atoms) were removed
the only force remaining would be the force from the atoms outside the shell (gray
atoms). For the black atom to be at equilibrium, the traction due to atoms inside the
shell (wide arrow) must cancel out the traction from the atoms outside the shell. Thus
the traction across the surface of the shell due to the vacancy is negative the force on
this atom from atoms outside the shell.
c) Simulation techniques
So far an expression was obtained for the dipole as a function of positions and forces
extracted from atomic simulations. The question of the choice of the technique to use in
atomic simulations to obtain forces remains. We now introduce several atomic
simulation techniques and compare their strengths and weaknesses.
The families of representations of materials are ab initio, tight-binding and empirical
FIG. 3.4: Force on an atom belonging to the shell (black
atom) from the atoms outside the shell (gray atoms) and
“force from the vacancy” (wide arrow).
potentials. In ab initio simulations, the Schrödinger equation is solved (under some
assumptions) [Kohn and Sham 1965, Kohn 1999]. These calculations are intrinsically
quantum mechanical, which makes them very accurate. However they are
computationally intensive which prevents the simulation of large systems. Empirical
potentials eliminate the electronic degrees of freedom. The force from one atom on
another atom is calculated as a function of their separation distance and the location of
surrounding atoms. The expression for this potential is not theoretically derived but
some insight from quantum mechanics may be used in motivating these expressions.
Empirical potentials have parameters which are fitted to the established properties of the
material of interest (known experimentally or from ab initio calculations). As a result,
while the lattice parameters and cohesive energies are outputs of ab initio calculations,
they are inputs for empirical potentials. Empirical potentials can be considered to be
mostly interpolations between known properties of the material in question (relative
energies of crystal structures, elastic properties, etc.) Therefore predictions which rely
on aspects of the potential far from the fitting regime are not quantitatively reliable.
Tight-binding [Slater and Koster 1954, Goodwin et al. 1989] is another simulation
technique, it uses a very simplified quantum mechanical description of the atoms. This
makes these simulations simpler to implement, less computationally-intensive but also
less accurate than ab initio calculations. Their relative simplicity also allows for larger
systems than ab initio. Therefore, both in terms of system size and of accuracy, tight-
binding (TB) is intermediate between empirical potentials and ab initio.
Stillinger and Weber [Stillinger and Weber 1985] designed an empirical potential to
study the melting of silicon. Due to the covalent nature of silicon bonds, a mere two-
body term does not suffice because the energy would then be proportional to the number
of bonds which would drive the system to a close-packed structure. Stillinger Weber
(SW) potential uses both two-body and three body terms:
Φ = ∑ v 2 (rij ) + ∑ v (r , r3 ij jk , θ jik ) . (3.32)
i< j i < j< k
The first summation is over pairs of atoms and the second is over triples. For a given
pair of atoms, the two-body term depends only on the distance r between the atoms,
⎡ ⎛ r ⎞ −4 ⎤ ⎛ 1 ⎞
v 2 (r) = ε A ⎢B⎜ ⎟ − 1⎥ exp⎜ ⎟ (3.33)
⎦ ⎝r/σ −a ⎠
where ε, A, B and σ are positive constants. The exponential term drives v2 to 0 when r/σ
approaches the constant a from below. σa is therefore a cut-off distance. Equation (3.33)
applies when r/σ < a and v2 is set to 0 when r/σ > a. The value of a is chosen such that
the cut-off occurs between first and second nearest neighbors, as a consequence there is
no two-body interaction between second nearest neighbors. Whereas, physically, atoms
further apart contribute to the energy limiting two-body interactions to first nearest-
neighbors simplifies the relationship between the model parameters and many properties
such as lattice parameters and bond lengths for various crystal structures, elastic
constants. This greatly simplifies the routine to optimize the parameters.
r j θjik
FIG. 3.5: The two-body terms only depend on the
interatomic distance while the three-body terms also
account for the angle between the bonds.
The three-body term models aspects of the sp3 bonding that cannot be adequately
described by two-body interactions. In this term the energy depends both on distances
and angles, as shown in Fig. 3.5,
v 3 (rij , rik , rjk , θ ijk ) = ε h (rij , rik , θ jik ) + ε h (rji , rjk , θ ijk ) + ε h (rki , rkj , θ ikj ) (3.34)
⎛ γ γ ⎞⎛ 1⎞
h (r1 , r2 , θ ) = λ exp⎜
⎜ r / σ − a + r / σ − a ⎟⎜ cosθ + 3 ⎟
⎝ 1 2 ⎠⎝ ⎠
and λ and γ are positive constants. Again the exponential plays the role of a cut-off and
h is zero when r1 or r2 is greater than σa. Notice that in the case of a perfect diamond
cubic crystal, cos θ = -1/3 due to the tetrahedral symmetry and the three-body terms do
not contribute to the energy.
When an atom is removed to form a vacancy, its first nearest-neighbors can relax
(generally inward). Different simulation techniques predict different amounts of
relaxation and different formation energy. Table 3.1 shows the range of formation
energy of a vacancy and of the radial component of the displacement of the first nearest
neighbors from experiment, ab initio, tight binding, Stillinger Weber and other
empirical potentials. Space group Td corresponds to a radial displacement of the first
nearest-neighbors while in D2d there is a pairing of nearest-neighbors which form two
dimers with the distance between the two atoms of a dimer smaller than the distance
from atoms of the other dimer. The formation energy obtained by ab initio calculations
is not very wide-ranged and is consistent with experimental results. The displacement of
the first nearest neighbors, on the other hand, can vary greatly (by a factor of two.) In ab
initio simulations for instance it varies between -0.48 Å and -0.22 Å. Pushka and
coworkers also found the symmetry to be either D2d or Td depending on the size of their
system [Pushka et al. 1998]. This indicates that energy converges faster than geometry
and that geometric data, such as formation volumes, cannot be obtained with small
systems. According to empirical potentials, the first nearest neighbors may move
inwards or outwards. These simulations are the least reliable because the potential are
fitted to perfect crystals and therefore poorly model the changes in bonding near a
technique references space energy (eV) displacement (Å)
experiment Watkins 1964; Dannefaer 3.6 ± 0.2
ab initio Antonelli 1989, 1998; Zhu D2d* 3.3 → 3.65 -0.48 → -0.22
1996; Puska 1998; Zywietz
tight Song 1993; Lenosky 1997; D2d 3.68 → 5.24 -0.50 → -0.42
binding Tang 1997; Munro 1999
SW Stillinger and Weber 1985 Td 2.82 - 0.56
other Balamane 1992 Td 2.82 → 3.70 -0.51 → +0.24
Table 3.1: Formation energy of a vacancy and displacement of the first
nearest neighbors from experiment, ab initio, tight binding, Stillinger Weber
and other empirical potentials. *: there exist a few reports of Td symmetry.
Any technique, be it experimental or computational, has limitations. It is therefore
not always possible to use only one technique. Simulation techniques can be limited in
two ways: accuracy and computational cost. The most accurate techniques being the
most computationally intensive, they are limited to small systems. Computationally less
intensive techniques on the other hand are not efficient far from equilibrium, in
particular where the lattice is distorted (defects, surfaces.) Multiscale modeling of
materials aims to bring two (or more) different techniques together, each providing its
specific strength(s) and compensating for the weakness(es) of the other technique. One
possibility is to use several techniques within the same simulation: ab initio is used
where accuracy is needed and an empirical potential is used where structural changes
are not expected to occur. This provides a means to increase the system size without
increasing the computational cost significantly. A slightly different kind of simulation
uses atomistics close to a singularity (crack tip, defect, indenter) and continuum
mechanics for the rest of the system [Shilkrot et al. 2002].
a) Atomistic results
The dipole tensor, D, gives the magnitude and anisotropy of the center of contraction
and cannot be obtained by elasticity, but must be determined by the microscopic
structure of the point defect. A number of different techniques have been used to
characterize the relaxation around a point defect. One typical method is to note the
relaxation of the nearest neighbor atoms. However this method is not effective for
describing the asymptotic elastic relaxation in the vicinity of the defect, which is
important for accurately calculating the relaxation volume, i.e. the quantity necessary to
predict the thermodynamic response of the defect to stress. We detail here a systematic
method for extracting the relaxation around the vacancy. One method to obtain D would
be to fit the displacement curve as a whole to the asymptotic elastic solution. While this
is feasible it is not an efficient way to proceed and involves fitting the curve in regions
close to the defect and close to the periodic boundary where the solution in an infinite
medium cannot be expected to apply. Rather we obtain D from Eq. (3.31), i.e. we find
the value of the dipole that provides a best fit to the forces obtained form atomistics.
b) Isotropy of the vacancy in silicon
Equations (3.9) to (3.31) make no assumptions as to the isotropy of the dipole
although (3.16) to (3.31) do assume an isotropic elastic medium. Equilibrium only
requires that the tensor be symmetric to ensure that there is no net moment. However,
conjugate gradient (CG) calculations show that the actual dipole of a vacancy, as may
be expected, is nearly isotropic. Figure 3.6(a) shows the ratio of off-diagonal term of D
to diagonal terms of D. Far from both the vacancy and the boundaries the dipole is very
close to being diagonal. At any shell the non-diagonal terms are never more than a few
percent of the diagonal terms. Figure 3.6(b) shows the standard deviation for the
diagonal terms of D normalized by the trace of D as a function of the shell where D is
calculated. When D is calculated far from the vacancy the standard deviation is less than
0.1 % of the trace and the three diagonal terms are essentially equal. Thus for shells far
enough from the vacancy, the dipole is nearly proportional to the identity tensor. An
example of such a tensor (in eV) is
⎛ 8.506 3.2x10 -3 − 1.7 x10 -3 ⎞
D = ⎜ − 9.4x10 -3 8.501 − 5.4x10 -3 ⎟ . (3.36)
⎜ − 0.2x10 -3 − 2.4 x10 -3 8.506 ⎟
Therefore, we can write the dipole as
where D is a scalar and I is the identity tensor. In what follows, when we refer to the
dipole, we will be referring to the scalar D.
FIG. 3.6: The ratio of off-diagonal terms of D to diagonal terms (a)
and the standard deviation for the diagonal terms of D (b) as a
function of the shell where D is calculated. Plotted for 512, 1 728,
4 096, 8 000, 13 824 and 32 768 atoms.
c) Displacement field and formation volume
Once extracted the value of the dipole can be used to calculate the formation volume.
The simplest case to calculate is an isotropic elastic sphere of radius R, where the radial
displacement is given by the expression:
D ⎡ C11 − C12 ⎛ r ⎞ ⎤
u r (r ) = ⎢1 + 2 ⎜ ⎟ ⎥. (3.38)
4π r 2 C11 ⎢
⎣ C11 + 2C12 ⎝ R ⎠ ⎥⎦
While the first term arises directly from the asymptotic elastic field from Eq. (3.16), the
second term is imposed by the free boundary at R. From Eq. (3.38) it follows that the
measured formation volume is related directly to the displacement at the outer boundary
V f = 4π R 2 u r (R ) = . (3.39)
C11 + 2C12
Note that Vf is independent of R. For a large system, where continuum elasticity applies,
the formation volume is independent of the size of the system. Since a large cube should
not be different from a large sphere, Eq. (3.39) is expected to hold for any isotropic
system where finite size effects can be neglected, independent of geometry.
The dipole values that were obtained from a series of conjugate gradient calculations
using the Stillinger-Weber model ranging in size from 512 atoms to 32 768 atoms. The
value of D was calculated on concentric shells around the defect. The shell of first
nearest neighbors of the vacancy is not used: since there is nothing strictly inside this
shell, the external force is 0 at equilibrium. Shells too close to the vacancy show
evidence of discreteness effects. This is to be expected since continuum elasticity does
not apply down to the atomic scale. Ten samples were used for each system size except
the larger ones since they were more computationally-intensive. In some cases the
simulations converge to distinct vacancy structures with different formation energies,
FIG. 3.7: Dipole values as a function of the cubic shell at which
the force data is extracted for 30 samples made of 4 096 atoms.
different formation volumes and different dipole values. Figure 3.7 shows the value of
the dipole as a function of the shell where it is calculated for 30 samples made of 4 096
atoms. There are two kinds of curves corresponding to two structures of the vacancy.
Within each structure there exists some variation of the properties. Only simulations
leading to the lowest energy structure were considered to plot the figures (other than
Fig. 3.7) in this chapter. In all figures bearing error bars, the error bars are sample-to-
sample variations among the samples of the lowest-energy structure. Therefore they do
not account for systematic errors due to system size effects. Table 3.2 shows the number
of lowest energy samples obtained for each system size.
system size 512 1 728 4 096 8 000 13 824 32 768
number of samples 10 10 10 10 6 4
Table 3.2: Number of sample used for each system size.
Figure 3.8(a) shows the dipole values as a function of the shell at which it is
calculated. Figure 3.8(b) shows the dipole as a function of the shell over shellmax, where
shellmax is half the vacancy-vacancy distance. Thus shell/shellmax varies between 0 at the
FIG. 3.8: Dipole values as a function of the cubic shell at which the data are
extracted (a) and as a function of the ratio of the shell to the largest shell (b).
Each shell is numbered by the distance that separates the closest atom in the
shell from the vacancy. The error bars are from sample-to-sample standard
deviation. Plotted for 512, 1 728, 4 096, 8 000, 13 824 and 32 768 atoms.
vacancy and 1 at the boundary of the simulation cell. The fact, shown in Fig. 3.8(b), that
the curves for different systems sizes are close together far from the vacancy is an
indication that linear elasticity applies there. The error bars correspond to sample-to-
sample standard deviation. The shell of the first nearest neighbors was not plotted as
indicated above and the shell of second nearest neighbors gives a very high dipole due
to finite size effects. The third to fifth shells give a fairly low dipole value, again a finite
size effect. The sixth shell and above form a plateau where the dipole is almost constant.
For shells further out, the boundary has an increasingly important influence and the
dipole decreases. The sixth and seventh shells will be used to extract the dipole because
they are the smaller shells without finite size effects. For small systems, 512 and 1 728
atoms, there is no evident plateau since there is no region far enough from both the
defect and the boundary.
We can now use the dipole extracted from the atomistic simulations to obtain the
formation volume from Eq. (3.39) and Stillinger Weber elastic constants. This volume is
plotted in Fig. 3.9 along with the direct measurements of the change of volume of the
simulation supercell. The calculated formation volume does not match the relaxation of
the simulation cell. The reason for this discrepancy is that the calculated formation
volume assumes that the system is isotropic. Since there is no closed-form expression
for the stress field in the anisotropic case a fully anisotropic calculation would be much
more complicated. In the next sections a method will be discussed to correct for
anisotropy when calculating the dipole value from isotropic equations.
FIG. 3.9: The formation volume versus the system size measured both using Eq. (3.39)
(solid line) and from direct measurements of the change of volume of the simulation
supercell (dashed line). The error bars correspond to sample-to-sample standard
deviation; they do not account for systematic errors.
d) Finite element calculations
In order to correct for the assumption of isotropy made in Eqs. (3.29) and (3.30) it is
necessary to calculate a value of D/Vf appropriate for determining the formation volume
in the anisotropic medium given the dipole extracted assuming an isotropic medium.
This has been addressed by a series of finite element (FE) calculations in which the
stress field around the defect was obtained and related to the volumetric relaxation of
the box [Bouville et al. 2004D]. Obtaining the relationship between the extracted dipole
and the formation volume required a convergence study of the solution with respect to
the refinement of the discretization. The constitutive behavior of the mesh was taken
from the anisotropic (cubic) elastic moduli of the Stilinger Weber potential [Balamane
et al. 1992].
FIG. 3.10: Relaxation volume as a function of the number of elements.
The vacancy was modeled by a cube-shaped hollow region of dimensions 1/48 x 1/48
x 1/48 of the system size located at the centroid of the mesh. The dipole was represented
by point forces, directed toward the origin, applied at the centers of the inner faces of
this cube. With the points of application of these forces being known, their magnitudes
were specified such that the dipole strength was 1 nN.Å (= 0.624 eV). For the dipole to
be equivalent to forces applied at the first nearest neighbors of the vacancy, this
corresponds to a system of dimensions 12 x 12 x 12 unit cells. The outer surfaces of the
cube were allowed to relax inward while maintaining the planarity of the surfaces. The
extent of this relaxation was varied until corresponding normal force on each outer face
vanished. These boundary conditions were easier to implement than periodic ones, and
were therefore preferred. They resulted in displacement fields for which the relaxation
volume differed by less than 10-2 Å3 from the fields for periodic boundary conditions.
Since the dipole is an elastic singularity and the cubic shape introduces further stress
concentrations, the finite element solutions were slow to converge with mesh
refinement. This necessitated considerably fine meshes. Figure 3.10 shows the
relaxation volume as a function of the number of elements. If the number of elements is
6N3, the number of nodes is 6(N+1)3 - 12(N+1)2.
The three-dimensional stress tensor obtained at element quadrature points with each
mesh was projected to the nodes of the mesh using a least-squares formulation. The
radial stress component at each node was then obtained. The slow convergence rate
applies to these stresses also. Finite element error analysis predicts that the stress
projected to the nodes converges at the rate
|σnode - σexact| ≤ C h2, (3.40)
where h is the element size and C is a constant [Hughes 2000]. The same is true of the
volume. Thus using the results from two mesh sizes the asymptotic value can be
⎛ h1 ⎞
⎜ ⎟ V2 − V1
V≈⎝ 2⎠ 2 . (3.41)
⎛ h1 ⎞
⎜ ⎟ −1
Figure 3.11 shows the volume obtained from Eq. (3.41) where the size of mesh 2 is
constant (6x563 elements) and the size of mesh 1 is on the x axis. This shows that,
unexpectedly, Eq. (3.41) does not provide an asymptotic value independent of the
choice of the meshes. This is because convergence is very slow for finite element
calculations with a singularity. The stresses have the same problem.
FIG. 3.11: The volume obtained from Eq. (3.41) where the size
of mesh 1 is the x axis and the size of mesh 2 is 6x563.
Figure 3.12(a) shows the output dipole per unit input dipole as a function of the shell
where it is calculated for five finite element meshes. The curves for the finer meshes
have similar shapes and they are similar to what was observed atomistically (Fig. 3.8).
However the magnitude of the dipole is different for the different meshes due to the lack
of convergence. The high values close to the defect are due to finite size effects and the
fact that the dipole was implemented as force pairs a finite distance apart.
Equation (3.39) provides a relationship between the formation volume and the dipole
for a sphere of radius R made of an isotropic material. However the proportionality
constant applies only to an isotropic medium. In an anisotropic medium the formation
volume is also of the form Vf = K D but in this case the proportionality constant K is
unknown. Since both atomistic and finite elements results follow this relationship,
= . (3.42)
D FE D at
FIG. 3.12: Ratio of the output dipole to the input dipole (a) and to the relaxation volume
in eV/Å3 (b) as a function of the cubic shell at which the data is extracted from finite
element calculations. Closed circles: 6x63 elements, open triangles: 6x123, closed
diamonds: 6x243 elements, crosses: 6x363 elements and open squares: 6x483 elements.
The thick solid line in (b) is an extrapolation.
f f f
In order to obtain Vat from Dat, only the ratio VFE / D FE is needed. Although VFE and
DFE converge slowly their ratio may not. Figure 3.12(b) shows the ratio of the output
dipole to the volume, D FE / VFE , as a function of the shell. Unlike the volume and the
dipole taken separately, the ratio is nearly converged. The two curves are closer together
than those in Fig. 3.12(a). Figure 3.13 shows DFE as a function of VFE for five different
mesh sizes. D FE / VFE is almost independent of the mesh although VFE and DFE are not
The medium used in the FE calculations is anisotropic. The dipole was extracted
from the FE calculations using Eqs. (3.29) through (3.31). Thus the error introduced in
the results shown in Fig. 3.8 by the use of Eqs. (3.29) through (3.31), which assume an
FIG. 3.13: DFE (calculated at the shell situated at 0.45) in
eV as a function of VFE in Å3 for five different mesh sizes:
6x63, 6x123, 6x243, 6x323 and 6x483. The dotted line
shows that D FE /VFE is almost constant for the larger shells
6x243, 6x323 and 6x483 (filled symbols).
isotropic medium, also exists in the results relating the dipole value to the formation
volume shown in Fig. 3.10. Since the FE results are used to derive a formation volume
from the dipole extracted in this way it is reasonable to expect that the errors cancel out
and the formation volume obtained no longer includes a systematic error arising from an
assumption of isotropy.
Since D FE / VFE is close to convergence, Eq. (3.41) can be applied to it. Figure 3.14
shows the result for D FE / VFE (in eV/Å3) thus obtained. The dotted line is a power law
fit to the part of the data far enough from the vacancy for finite size effects to be
neglected. Its equation is
⎛ shell ⎞
D FE / V
FE = 0.47 − 0.59⎜
⎜ shell ⎟
⎟ . (3.43)
⎝ max ⎠
At the defect, D FE / VFE ≈ 0.47 eV/Å3, as opposed to 0.67 eV/Å3 in the isotropic case.
FIG. 3.14: D FE / VFE (in eV/Å3) from finite elements as a
function of the shell at which the data is extracted. The dotted
line is a power law fitted to the data far from the vacancy.
e) System size effects
Figure 3.15(a) shows as a function of the system size the values of the formation
volume obtained from the dipole and of the formation volume calculated by directly
measuring the change in volume of the supercell upon the introduction of the defect to a
FIG. 3.15: The formation volume as a function of the system size (a) and of 104
over the system size (b). Solid line: volume calculated using the dipole; dotted
line: direct extraction from atomistic simulations. The error bars correspond to
sample-to-sample standard deviation; they do not account for systematic errors.
system held at zero pressure. Figure 3.15(b) shows the formation volume as a function
of 10 000 over the system size. If there is convergence, the formation volume for an
infinitely large system can be read at the intersection between the curve and the y-axis.
The volume obtained through the dipole converges to a value of 15 Å3 while the direct
measurement gives 13.8 Å3.
Accurate calculation of formation volumes from atomistic models is important for
modeling stress-defect interactions during diffusive processes. The Stillinger Weber
potential was used because it allows for the simulation of larger systems than quantum
mechanical methods. We presented a new method which calculates the formation
volume by matching stresses near the defect to the asymptotic elastic prediction. This
method has been shown to converge with system size to a value close to that obtained
by measuring the change in volume of the simulation cell. This validates the new
method presented in this chapter. It is now possible to find the elastic field around the
defect given Vf. This will enable the simulation of real systems by superposing the
stress field surrounding the individual defects.
As shown in table 3.1, the Stillinger Weber description of the vacancy is not
quantitatively accurate. In order to obtain quantitatively accurate results a better
description of silicon is necessary close to the vacancy. However, this improvement in
model accuracy should not happen at the cost of a dramatic shrinkage of the system size.
Two possibilities are available. One could use tight-binding which is more accurate than
empirical potentials but not as computationally intensive as ab initio, the description of
the vacancy is fair and the system can be simulated using thousands of atoms. This
approach is not efficient because tight-binding is used far from the vacancy where an
empirical potential would be good enough since only the correct elastic properties are
needed. Another solution is then to use ab initio (or tight-binding) methods close to the
vacancy, where the system is far from the equilibrium structure, and an empirical
potential further away where computationally-intensive methods are not necessary.
A full-scale simulation of diffusion in semiconductors would require data on other
point defects, interstitials, substitutionals, vacancy-interstitial pairs and other defects
[Goedecker et al. 2002] since all of these defects can exist and interact in the devices.
The methodology we developed can be applied to these defects, with some
modification. These methods may also be applicable to other kinds of crystal defects,
such as dislocations [Shilkrot et al. 2002] or more generally to any material
inhomogeneity leading to a singularity in the stress field. We applied this methodology
to silicon, but it is general enough to be applied to other materials.